Optimization of Wear Process Parameters of Al6061-Zircon Composites Using Taguchi Method

Aluminium metal matrix composites are utilised extensively in a variety of engineering applications, including those involving automobiles, aerospace


Introduction
Due to the obvious growing need for lightweight and highperforming materials in recent years, the focus of research has turned away from monolithic materials and toward composite material systems.Due to the superior mechanical and tribological characteristics that aluminium and aluminium alloys possess in comparison to base alloys, they have become increasingly popular in recent years as a result of their application in a variety of industries.Due of its light weight, high specifc strength, excellent stifness, and superior wear resistance, in particular aluminium-based particle reinforced multimaterial composites (MMCs) are gaining widespread acceptance.As a result, it fnds the applications as of all-purpose production industries infavour of aerospace applications.For the optimum combination of favourable mechanical qualities, good formability, and strength, the aluminium alloy 6061 is the best choice among the many other series of aluminium alloys that are currently available.When compared to alternative processing techniques, the stir casting technique is discovered to be both simpler and more cost-efective as a manufacturing method.Tis is especially true when discontinuous reinforcements are utilised in the process.It is possible to achieve homogeneous dispersion by frst preheating the reinforcement in a graphite crucible while ensuring that the environment is inert and using a two-step stirring operation.After conducting research into the impact of the size of particle and weight percentage on the wear properties of aluminium MMCs, the researchers arrived at the conclusion that sliding distance and load were the two criteria that were the most crucial to consider.Te use of ultrasonic vibration on the composites during melting resulted in a more refned grain microstructure of the produced composite, as well as enhanced mechanical and tribological characteristics of the fabricated composite.Te processes used in the production of MMC play a signifcant part in the enhancement of the material's mechanical and tribological characteristics.Powder metallurgy, friction stir processing, stir casting, and squeeze casting are only some of the techniques that have been developed for the synthesis of the particle reinforced aluminium matrix composites (Al MMCs).Te stir casting method was considered to be the easiest and most costefective approach for the development of composites, according to both the professional opinion and the literary portrayal of the abovementioned processes and procedures.Te actual process of stir casting begins with the melting of the base metal in a furnace of some kind, and then the use of a mechanical stirrer to continuously combine the solid particles with the liquid metal that has been melted.Te stirrer is responsible for ensuring that the molten metal contains an even distribution of the particles.In stir casting procedures, the amount of time spent stirring is another factor that determines the quality of the fnal result.When dealing with reactions that are infuenced by multiple variables, the Taguchi strategy is the superior technique to use.For the purpose of developing Al MMCs with improved mechanical characteristics and superior resistance to wear, researchers focus on both the experimental and analytical aspects of these materials.Te frictional force was taken from DUCOM in order to determine the coefcient of friction, and the impacts of characteristics such as applied load and sliding distance were explored in order to determine how those parameters afected the response.
Te Taguchi method is a noteworthy method for the development of high-quality systems that depend on an orthogonal array, which is a trustworthy and methodical strategy for optimising designs in terms of performance, quality, and cost.In this case, the necessary number of experiments is represented as an orthogonal array.In the Taguchi experimental design method, there are fve fundamental phases that are applied.Phase 1 is the planning of the experiment, Phase 2 is the design of the experiment, Phase 3 is the actual experiment, Phase 4 is the analysis of the results, and Phase 5 is the confrmation of the prediction.A best collection of well-balanced (minimum) experiments can be obtained by the use of orthogonal arrays.An appropriate orthogonal array (OA) is selected for the process, taking into account the process parameters and the levels at which they are specifed and the tests are conducted in accordance with the OA's specifcations.Diferent orthogonal arrays exist."Te signal to noise (S/N) ratios, which are divided into three diferent categories of quality attributes, like lower is better (LB), higher is better (HB), and nominal is the best, are used to evaluate the experiment's outcomes."Te NB value is considered to be the best and this will be determined by how the process reacts; in this case, the reaction is wear, and since we want to minimise the response's value as much as possible, this will be the determining factor.LB characteristics will need to be used in this situation.Te mathematical equation that represents the smaller the S/N ratio, the better it is represented by the number 1.In addition, an analysis of variance, also known as an ANOVA, was performed in order to calculate which of the two parameters was more infuential than the other and how much of an impact each variable had on the total amount of wear.Both the S/N ratio and the ANOVA were utilised in order to locate the optimal parameter settings for the process.Following this, a confrmation test was carried out in order to establish beyond a reasonable doubt that these optimal combinations are, in fact, the most efective ones.
Following is a discussion of the literature review that has been performed out over the course of the past few years on the Taguchi method for optimising the wear process parameters of aluminium alloy-based composites.Mallik and Mallik [1] fabricated aluminium-based MMCs and optimised the wear parameters using the Taguchi technique.Tey found that "the applied load (59.04%), preceded by sliding distance (20.85%), and % of reinforcement had the biggest impact on the wear rate of hybrid MMCs (16.85%)."Bhaskar and Sharief [2] studied the wear characteristics of aluminium MMCs by utilising the Taguchi method.Tey came to the conclusion that with the deployment of DOE approach, sliding distance contributed 48.63 percent to the wear of composites, while load contributed 25.74 percent.
Sahin [3] studied on the production and wear characterisation of MMCs.Tey discovered that the size of the reinforcement was the most infuential parameter on the wear, preceded by the % of reinforcement.When comparing the projected wear resistance to the actual wear resistance, there was found to be an excellent agreement at the level of confdence of 95%.Prakash et al. [4] carried out the Taguchi implementation in order to optimise the adhesive wear properties of aluminium MMCs.Teir fndings showed a reduction in the wear rate of MMCs brought about by the addition of reinforcement in comparison to matrix alloy.Te rate of wear is shown to reduce with increasing sliding distance because of the smoothing out of asperities and the surface hardening that occurs at the surface.Sundaresan et al. [5] carried out the process optimization of aluminiumbased composites, and from the wear study, it was found that by implementing the analysis of variance, the reinforcement percentage and the sliding velocity have more contribution for the wear behaviour.Tis was discovered through the work that they did on the process optimization of aluminium-based composites.Sutradhar and Sahoo [6] 2 Advances in Materials Science and Engineering studied the wear characteristics of aluminium-based MMCs and carried out the optimization by using the Taguchi method.Tey came to the conclusion that the applied load (L) is found to impact the wear the most considerably, while speed (S) and time (T) have got some major infuence as well.Ranaa et al. [7] examined the process parameters impact on the wear rate of aluminium-based MMCs.Tey came to the conclusion that for the composites produced at temperature ranges of 700 °C to 750 °C, this was found to be the optimal condition.Researchers discovered that a lower stirring speed of 50 rpm led to an increase in wear rates.Sahoo and Sutradhar [8] conducted research on the production and wear studies of aluminium MMCs using an optimization technique.Tey discovered that the composite exhibited reduced wear when the reinforcing weight percentage was increased.When the load was raised, the rate of wear on the composites also increased.Mohana sundararaju et al. [9] conducted research on the optimization of wear characteristics of aluminium-based MMCs using the Taguchi technique.Teir fndings showed that the integration of reinforcing particles into the produced composites gave the material a stronger resistance to wear.According to the fndings, the load on wear rate and COF were the most important parameters to consider.Rana et al. [10] conducted research on the Taguchi implementation for aluminium-based composites.Tey observed that the load, followed by the sliding speed and the sliding distance, attributed most to the wear rate.Te error connected with the study is 3.9 percent, and the error related with the confrmatory test is 5.8 percent accordingly.Chandramohan and Davim [11] carried out the Taguchi implementation to study wear characteristics of MMCs, and they came to the conclusion that the wear resistance of the material increases when reinforcement particles are incorporated into the aluminium matrix.When it came to the wear of composites, the sliding distance was the wear parameter that had the most signifcant impact on the wear.Te main objective of the current research is to produce Al6061-Zircon particulate composites by using a two-step stir casting process and to carry out a pin-on-disc wear test at elevated temperature 100 °C.Te Taguchi orthogonal design is utilised to determine the wear using design factors such as Zircon's weight percentage (expressed as a wt.percent), load, sliding distance, and speed.For the purpose of determining the wear, a multitribo tester is utilised.Te Taguchi method is utilised so that the optimal combination of parameters may be determined, which in turn produces the optimal (or least) wear.Te purpose of conducting an analysis of variance is to determine the degree to which individual factors and the interactions between them are signifcant.

Materials and Experimental Details
2.1.Materials.In this study, the base metal was an aluminium alloy called Al6061 and zircon was employed as the reinforcing material.Aluminium alloy with a precipitationhardening number 6061, often known as Al6061, contains magnesium and silicon as its primary alloying components.It is very widely extruded and possesses excellent mechanical qualities.It also demonstrates excellent weldability.It is the most commonly used aluminium alloy, and its applications are extremely diverse due to its extensive use.Table 1 presents the fundamental elements that make up the Al6061 aluminium alloy.
Numerous rare earth elements, titanium minerals, monazite, and other minerals make up the majority of zirconium silicate (ZrSiO 4 ), along with a minor quantity of hafnium.Zircon was discovered to be an excellent potential option for use as a reinforcing material in composites based on aluminium, zinc, and lead.Table 2 shows the chemical composition of Zircon.
Table 3 shows the chemical composition of Zircon physical and mechanical characteristics of Al6061 and Zircon.

Fabrication of Al6061-Zircon Particulate Composites.
Te quantity of zircon particles was increased from 6 to 12 weight percent, with each increase being a step of 3 weight percent.In order to produce the Al6061-ZrSiO 4 composites, the stir casting method was utilised.A frst measured amount of aluminium Al6061 was kept in a crucible composed of silicon carbide, which was then put in a furnace (electrical resistance) operating at a temperature of around 750 degrees Celsius.After properly degassing the melt with solid hexachloroethane, zircon particles with a particle size of sixty microns were weighed and added to the vortex of the melting process at a temperature of seven thousand fve hundred degrees (C2Cl6).Reinforcing particles were preheated to a temperature of 2000 degrees Celsius before being added to the melt using a two-stage reinforcement mixing procedure.Tis was conducted before the particles were put to the melt.Tis technique of incorporating reinforcement into an Al6061 alloy matrix in two stages will result in an enhancement in both the wettability of the matrix and the hardness of the reinforcement.In addition to this, it assists in the even distribution of the particles.Continuous stirring took place before, during, and after the addition of zircon particles to the liquid.Te stirring speed was normally kept at 200 rpm during the whole composite production process.After fve minutes of stirring, molten metal containing particles was poured into a cast iron die measuring 150 mm in length and 20 mm in diameter.Te length of the die was measured in millimetres.It had been fve minutes since the stirring had begun.Ten, machining was carried out for the developed castings.Te developed composites were subjected to a wear test utilising a pin-on-disc machine.

Wear Testing Experimental Details.
Figure 1 shows the Ducom Pin-on-disc tribometer was utilised in the wear tests that were carried out.Te samples, which have dimensions of 8 millimetres in diameter and 30 millimetres in height, are forced up against a rotating steel roller.Te equipment is set up in such a manner that the revolving roller will take on the role of the counter face material, while the stationary plate will take on the role of the test sample.At one end of the loading lever is a counter weight, and at the other end of the lever is a loading pan that is hanged for the purpose of Advances in Materials Science and Engineering placing the dead weight.Te load sensor is located quite near to where the loading lever is pivoting.It is a multipurpose piece of equipment that was created to investigate wear under sliding conditions.Te majority of the time sliding takes place between a pin that is immovable and a disc that is turning.Even after the contact surface of the arm has worn away due to wear and tear, the arm will continue to remain in touch with the disc because of the load.Tis will continue to be the case even after the arm has been subjected to wear and tear.Tis arm movement generates a signal that is utilised in the process of determining the maximum wear, while the friction coefcient is constantly measured as wear increases.Tis allows the maximum wear to be determined.During this process, the predicted level of wear is determined.Electronic single-pan scale with a resolution of 0.0001 g is used to determine the weight of each sample both before and after the experiment.Tis was conducted after giving each specimen a thorough washing with acetone solution.Because of this, it is to calculate the amount of weight loss that had been sustained by each specimen.
Table 4 shows the levels and process parameters.A sliding wear test was carried out with a variety of parameters, including the applied weight, speed, sliding distance, and % of reinforcement, and these factors were varied across three distinct levels.On the basis of the run order that was determined using the Taguchi model, a total of 27 separate tests were carried out.Wear is the response that the model provides.In an OA, the frst, second, third, and fourth column are designated for applied load, speed, sliding distance, and % of reinforcement.Te fnal column is designated for the wear response.Te reduction of wear is the primary focus of this model.A tabulation of the responses was performed, and an analysis of variance was performed on the fndings (ANOVA).Table 5 shows the L 27 Orthogonal array with wear.It also shows the SEM micrographs of wear tracks of the matrix and composite.Tis represents the cavities and large grooved regions on the wear surfaces and particles have been pulled out due to the change from a mild to severe wear resulted by an increase in the sliding distance due to a greater plastic fow on the pin surface of the specimen.Te particle pull-out was due to the poor particle/matrix bonding.Te presence of groove on the wear surface was observed moving parallel to the sliding direction.Figures 3(b) and 3(c) show the deeper grooves with the larger delaminated area on the worn surface.It is seen clearly from the fgure the presence of adhesive wear during the sliding.

Response Table for
Wear.Te impact of each control component on wear was calculated with an S/N response table utilising MINITAB 16.1 Software.Tese control parameters included load, speed, distance, and weight percentage.Te control factor with the most signifcant impact is identifed by calculating the delta value and is defned as the disparity between the control factor's minimum and maximum S/N ratios.Te response of the S/N ratio for wear is provided in Table 6, which demonstrates that, out of all the parameters, Load has the most signifcant impact, preceded by speed, sliding distance, and Wt. % for the composites that have been manufactured.Table 6 also reveals that weight percentage has the least signifcant impact.
Figure 4 demonstrates that the optimal conditions for wear are Al 6061 with 9 percent Zircon.As a result, the optimal setting of control factors for a composite with improved wear resistance has been determined.
Figure 5 depicts the impact of control factors interacting with one another.It is common knowledge that interactions do not take place when the interaction plots lines are parallel to one another, whereas signifcant interactions between parameters take place when the lines cross one another.

Analysis of Variance.
Te analysis of the impact on wear caused by characteristics viz load, speed, sliding distance, and % of reinforcement was performed with an ANOVA.Troughout the entirety of the process, the investigation was carried out at a level of signifcance of 0.05 or lower at all times.
Te fndings of the ANOVA for wear as a reaction to the factors are presented in abovementioned Table 7. Te variable with the most importance was load, which contributed 52.22 percent of the total, followed by speed, sliding distance, and wt.%.As a result, this aspect demonstrates the signifcant development in the results.

Regression Analysis.
In order to calculate the data in accordance with the characteristics of the produced composites, regression analysis is utilised.Te regression equation is utilised in order to make projections regarding the wear taking into account the various elements.Trough the use of the multiple linear regression approached, it was possible to determine the correlation that exists between the control factors and the wear.Tese control elements include load, speed, sliding distance, and wt.% of reinforcement.Te wear is calculated using the following regression equation: WEAR � 87.3519 − 1.01667 LOAD + 0.0222222 SPEED + 0.000777778 SLI DISTANCE + 0.537037 PERCENT.
(1) Te normal probability graph for wear in microns is indicated in Figure 6.Tis graph indicates that the errors associated with the experiments are negligible as the points are nearer to the line.

Confrmation of Experiment.
Te goal of this last step in the DOE process is to validate the optimal amounts of the parameters that were selected earlier in the process.Experiments to confrm the fndings were carried out using the

Conclusions
Te following conclusions are drawn from this study's fndings: (1) A successful adaptation of stir casting was made to fabricate Al6061-6 percent Zircon, Al6061-9 percent, and Al6061-12 percent composites.(2) Zircon particles can be included into the Al6061 matrix to produce the composite material with an even higher resistance to wear than it already possesses.Tis is one of the contributing components that help make the composite more resistant to wear over time.(3) Te scanning micrographs of Al6061-Zircon composites show the presence of zircon particles.It also shows that the particles are distributed uniformly in the Al6061 matrix.(4) Te scanning micrographs of worn out surfaces of Al6061-Zircon composites show the presence of grooves on the wear surface moving parallel to the sliding direction.It also shows the deeper grooves with the larger delaminated area on the worn surface.
It is seen clearly from the fgure the presence adhesive wear during the sliding.(5) Based on the response table, it is seen that load has the most signifcant impact, preceded by speed, sliding distance, and wt.% for the composites that have been manufactured.Te load has the greatest impact on the wear (52.22 percent), preceded by the sliding distance (40.86 percent), speed (2.64 percent), and weight % (weight percent) (1.27 percent).( 6) Te regression equation was established for this investigation, and it was used to the problem of predicting the coefcient of friction developed in composites under intermediate conditions with a level of accuracy that was considered acceptable.

3. 1 .
Microstructural Characterization of Al6061-Zircon Composites.Figures 2(a)-2(e) show the SEM micrographs of Al6061 Matrix, Al6061-3% Zircon, Al6061-6% Zircon, Al6061−9% Zircon, and Al6061-12% Zircon at 500x magnifcation.Te distribution of the particles, secondary phases of Al 6061 alloy are visible in the SEM.Figures 2(b)-2(e) show the presence of Zircon reinforcement particles.Figures 2(b)-2(e) show the irregular shaped white needle like structures, which are formed during precipitation of Mg 2 Si during solidifcation of the MMC.Tese secondary phases increase the strength of the composite due to strong adherence at the grain boundary.Te black regions with tetragonal shape indicate the Zircon reinforcement particulates.Te distribution of these zircon particulates is uniform in the matrix.Figures 2(d) and 2(e) indicate the SEM images for 9% and 12% weight fraction of zircon particles reinforced Al6061/ Zircon composite with large Zircon portions.Te precipitate Magnesium Silicate is formed due to the reaction between Si and Magnesium.Te secondary phase aluminium silicate is formed due to the reaction between aluminium and silicon.

Table 3 :
Physical and mechanical characteristics of Al6061 and zircon.

Table 4 :
Levels and process parameters.

Table 6 :
Response table for wear.

Table 7 :
Results of ANOVA for COF.

Table 9 .
Te results of confrmatory test indicate that the errors associated with the experimental wear in microns and regression model Equation wear are negligible.

Table 8 :
Results of experiment.

Table 9 :
Results of confrmation test.